Wear, 135 (1990) 403 - 422 403
DEVELOPMENT OF A UNIQUE LABORATORY SCALE FLUIDIZED BED WEAR TESTING UNIT*
Lawrence Berkeley Laboratory, Un~uers~ty of California, Berkefey, CA (U.S.A.)
Electric Power Research Institute, Palo Alto, CA (U.S.A.)
Significant wastage of internal bed components in fluidized bed com- bustors has been widely experienced throughout the industry. A major probable contribution to heat exchanger tube wastage in bubbling fluidized beds is mechanical in nature. It arises from the impact of blocks of de- fluid&d particles thrown against tube undersides during either the passage of rising bubbles or the collapse of teardrop like voids that form periodical- ly under tubes. In an effort to investigate this process, isolated from other erosive or corrosive effects, a novel wear testing rig has been designed and built. This device simulates the particle block impact environment by the fast movement of a specimen rod vertically within a minimally fluidized bed. Data from initial room temperature tests indicate that rods exposed in the rig suffered losses which were similar in both m~nitude and circum- ferential distribution to those experienced by tubes in other cold model studies that utilized more conventional fluidized bed units. The worn surface regions of the tested metallic rods were composed of a relatively hard multilayered composite of bed material and base metal that resulted from deposition of fine particle fragments and considerable surface deformation. Removal of material from this composite probably occurred primarily through a process of three-body microabrasion. For pure aluminum, a secondary process of layer spallation was active at circumferential locations where an exceptionally thick composite layer developed.
Energy production from the fluidized bed combustion of coal has many advantages over conventional coal burning methods. A large reduction in emission of the pollutants NO, and SO,, as well as a high combustion efficiency and wide fuel tolerance, make fluidized bed combustion an attrac- tive technology. A major problem encountered in the burning of coal by this process has been the material wastage of heat exchanger tubes and other
*Paper presented at the International Conference on Wear of Materials, Denver, CO, U.S.A., April 8 - 14, 1989.
0043-1648/90/$3.50 0 Elsevier Sequoia~~inted in The Netherlands
components immersed in the fluidized bed. This wastage involves mechanical wear processes combined in some instances with corrosion. Operation of fluidized bed combustors (fbc) has resulted in widely ranging tube wastage rates varying from essentially none, to unacceptable levels of 1000 nm h--l or more [l]. This range suggests that wastage is not intrinsic to the fbc environment, but arises from design and operational characteristics.
1.1. Background When an evenly distributed flow of gas passes upwards through a bed
of solid particles at very low velocities, the particles remain stationary in the form of a packed bed, while the gas flows through interstices. If the flow is increased, the upward gas velocity (superficial velocity u,) becomes suf- ficient to levitate the bed material. The bed is then said to be fluidized, and the air velocity at which this occurs is known as the minimum fluidizing velocity umf. The minimum fluidizing velocity is dependent on the gas density, particle density, and particle size. As the flow is increased, the bed expands and becomes less dense as inter-particle spacing increases. At some point, increased gas flow results in instabilities within the bed leading to the creation of bubbles near the distributor that grow by coalescence and rise through the bed. In most fbc systems, where the coal and sorbent particles are larger than 400 pm, this instability exists immediately upon fluidization so that the minimum bubbling velocity u,~ is equal to umf. Within the bubbling regime, increasing u, leads to a more violent bubbling and resultant large pressure fluctuations until a transition into the turbulent fluidization regime occurs. In the turbulent regime, small voids form and disappear throughout the bed in a random manner; pressure fluctuations are corre- spondingly small. The majority of fbc operate under a bubbling regime.
1.2. Particle block hammering process Mechanical wear in bubbling fluidized beds may result from many
causes; some may be intrinsic to certain regimes in the fluidized bed environ- ment while others are related to design or operational aspects. These processes, which have been discussed by Stringer and Wright [Z], include both high velocity, dilute phase erosive conditions, and high particle loading, dense phase abrasive conditions. One process which may be a major intrinsic contributor to the wastage of horizontal heat exchanger tubes immersed in bubbling beds arises from the impact of blocks of essentially defluidized particles on the underside of tubes. Experiments with cameras situated inside clear tubes have shown such particle blocks hammering tube bottoms with great force, and then dropping away or sliding upward across their surfaces . External viewing through clear bed walls has indicated that these impacts are associated both with the wakes of rising bubbles and the collapse of teardrop like voids that form periodically beneath tubes [ 41. Rising bubbles and the resulting particle blocks typically have a velocity of between 1 and 2 m s-l. Both bubbles and teardrop voids occur at a frequency of between 1 and 3 Hz. Peak forces on tubes associated with these block im- pacts have been measured to be in the range 50 - 800 N  dependending on bed dimensions and fluidizing characteristics.
The experimental evidence thus suggests that instead of individual bed particles freely striking the tubes, a particle is constrained to be in sliding contact with the tube for some time, loaded onto the surface by the block of unfluidized particles of which it is a member. This implies an abrasive wear process, rather than an erosive process. The particles appear to have some limited ability to move and rotate relative to one another and to the tube surface, which is consistent with a three-body abrasive process. Actually, it may well be that the true wear process includes aspects of both erosion and abrasion; more detailed analysis of the wear process is beyond the scope of this paper. The aim of this research is to study that part of the tube wear associated with the impact of blocks of particles, either in the wakes of bubbles or resulting from the collapse of teardrop voids.
1.3. Actuated specimen rig In an effort to investigate this process, isolated from other effects,
and in a controlled environment, a small fluidized bed unit has been designed and built with the unique feature of a horizontal specimen rod that can be quickly moved a short distance vertically within a minimally fluidized bed. The downward specimen motion is controlled to produce similar frequencies and velocities as those of the impacting particle blocks observed in bubbling fluidized beds. The resulting measured impact force is also similar to that which has been measured in real systems. Since the bed is minimally flu- idized during testing, all other contributions to wear are essentially elim- inated .
The actuated specimen test rig overcomes problems associated with conventional fluidized bed wastage testing units involving high cost and limited control. To recreate the environment typical of bubbling fbc, a flu- idized bed wear testing unit would need to be rather large (>0.6 m X 0.6 m) so as to overcome wall effects and to allow small bubbles the opportunity to coalesce into potentially more damaging larger ones. The maximum available fluidizing velocity would need to be as high as 2 m s-l. In such a large unit, control of temperature and local fluidizing behavior is difficult. Moreover, these conditions would require a large capacity air blower, capable of 1 m3 s-l, and some means of introducing around 250 kW in order to achieve fbc temperatures of 600 C. Since the laboratory rig relies on speci- men motion to simulate interactions with bubbles or teardrop voids, it can be operated at umf, essentially eliminating the effects of wall proximity and long-range flow patterns. The rig is thus scaled to accommodate the selected specimen size and to assure realistic fluidizing conditions. The required flow rate for the rig is 0.015 m3 s-l. A 4 kW external furnace is all that is necessary to heat this unit, making it possible to determine the temperature dependence of the wastage. In this paper, two tasks designed to qualify the rig cold by comparison with tests in large cold model fluidized beds are described. Investigations at elevated temperature will be presented elsewhere.
2. Experimental apparatus
A schematic of the fluidized bed wear testing rig is shown in Fig. 1. Dimensions and other characteristics are listed in Table 1. The body of the unit consists of a 155 mm diameter enclosed vertical cylinder that is partially filled with bed material. Quartz with a mean particle diameter of 800 pm was the material chosen in this study because it is often a major constituent of the inert bed material within fbc, and is believed to be primarily re- sponsible for component wear. Air is fed to a distributor within the bed consisting of four tubes extending radially from a central supply tube. Each tube extension has two holes on its underside. When in operation, air enters the bed via the eight distributor holes, flowing first downward and then uniformly upward through the bed towards the exhaust at the top, where it passes through a cyclone that collects escaping particle dust. The bed material, a few centimeters below the distributor, is not penetrated
C Pressure Probe
Fig. 1. Schematic diagram of actuated specimen fluidized bed wear testing rig.
Fluidized bed characteristics and ranges of operating conditions
Fluidized bed dimensions
Bed diameter 155 mm Bed depth range 102 - 914 mm Specimen dimensions 108 mm long x 19 mm diameter
Ranges for fluidizing and actuation characteristics
Number of holes 8 Hole diameter 4 at 4.0 mm, 4 at 4.4 mm Pressure drop 6.9 kPa (1 psi) at 0.50 m s-
Fluidizing velocity 0.25 - 1.25 m s-l Maximum specimen velocity 0.8 - 2.0 m s-l Specimen actuation frequency 0.27 - 2.8 Hz Specimen actuation amplitude 0 - 20 mm full deflection
by the air jets and thus remains in the packed condition. Typical distributors sit at the bottom of the bed and have orifices directed upward. The down- ward directed orifices of this rig prevent jet streaming, and thus allow the specimen to be situated close to the distributor. This design also helps prevent orifice blockage which can result in preferential bubhle paths and uneven fluidization. By adjusting the height of the distributor, the bed depth can be altered.
The specimen is a rod of circular cross-section, held horizontally in a stirrup on the end of an actuator rod within the fluidized portion of the bed. Specimen orientation is maintained with a locating pin. The specimen rod is driven downward within the fluidized bed at high accelerations by a pneu- matic air cylinder. The force of the downward stroke is altered by adjusting the air pressure supplying the cylinder. The bed material immediately below the moving specimen is compressed, or defluidized, and therefore behaves like the defluidized material that is thrown against the tube bottom during bubble passage or teardrop void collapse in bubbling fbc. The specimen accelerates at an approximately constant rate from its rest position at the top of the stroke to the stroke end. Typical values for this acceleration range 60 - 170 m s-*. The characteristics of the downward specimen motion were modeled after those of rising bubbles and collapsing teardrop voids. Maximum downward specimen velocities, like those of rising bubbles, are in the range 1 - 2 m s-l. The actuation frequency can be set between 0.27 and 2.8 Hz, similar to the measured pressure and tube force pulses of 0.5 - 3 Hz. The stroke length can be set between 0 and 20 mm. This is in the range of the observed teardrop dimensions of 10 - 50 mm. The return stroke is damped to prevent any significant wear occurring during the upward stroke since the system is meant to simulate particle blocks that impact the tube bottom only. The downward specimen motion typically takes between
10 and 15 ms for a 10 mm stroke. The specimen spends the remainder of the cycle time stationary at the ends of the stroke, or being slowly drawn to the top of the stroke.
Specimen motion is monitored through a linear v~~abled~s~~aceme~t transducer (LVDT) attached to the actuating rod. The force of particle blocks impacting the rod surface is determined via strain gauges that are mounted on a reduced section of the actuating rod. Pressure transducers are linked to probes that can be inserted into the bed through side ports located at intervab along the tube. These probes are used to determine the onset of flu~dization and to detect any bubbl~g that occurs within the bed,
3, Operational characterization
3.1. Bed particle conditioning During the first several hours of ~~~d~~ bed operation with fresh bed
material, nearly 20% of the quartz was reduced to fines and elutriated. This was found to be due more tu the rounding of particles by the cracking off of corners than to bulk fragmentation. After this initial period, the particles reached a relatively stable shape and size, and further elutriation was reduced to fess than 1% over 20 h. Changes in particle shape during testing are un- desirable, not only because of the possible chat particle abrasivity, but also because the associated change in particle size d~~ibution alters the state of fluidization. Accordingly, all tests were carried out with bed material that had been preconditions in the fluid&d bed. F~h~ore, the finer bed material that had naturally levitated to the top of the bed during fluidization was vacuumed off and replaced with fresh material between test increments. These procedures yielded bed material that was of a satisfactorily consistent size and shape distribution over a time in excess of 1000 h. A typical coliec- tion of conditioned quartz particles used during testing is shawn in the scanning electron micrograph in Fig. 2.
Fig. 2. Catlection of typical conditioned quartz partkles used in fkidized bed wear study.
3.2. Fluidking behavior The wear rate was found to be strongly dependent on the excess flu-
idizing velocity (u,, defined as u, - ZQ). It is therefore important that U mf be determined precisely, and that u, be set and monitored accurately. The preferred method for determining the onset of fluidization is to monitor the pressure drop across the bed as u, is increased . The press...